This specification covers measurement of strain resistance of anodic coatings on aluminium and its alloys, that have undergone a sealing treatment and contact with an acidic solution, are stainproof or nonadsorptive with respect to dyes. The method comprises contacting the test area of the anodized specimen with nitric acid solution and, after rinsing and drying, applying a special dye solution followed by rinsing and rubbing the test area with pumice powder, drying, and visual examination of the test area for retention of dye stain. Coatings that exhibit no dye stain or change in color are considered to have passed the test. Reagent grade chemicals shall be used in all tests. A specified solution of nitric acid shall be prepared in distilled or deionized water. A specified volume of aluminium blue 2WL dye shall be dissolved in distilled or deionized water.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This method is intended to determine whether anodic oxide coatings on aluminum and its alloys, that have undergone a sealing treatment and contact with an acid solution, are stainproof or nonadsorptive with respect to dyes.
1.2 Coatings that have been properly sealed should be proof against adsorption of coloring materials and, hence, “nonstaining” in many types of service.
1.3 This method is applicable to anodic coatings intended for applications where they are exposed to the weather, or for protective purposes in corrosive media, and where resistance to staining is important.
—Performance in this test is predictive only of susceptibility to stain by dyes. It is not intended to be predictive of other factors in service performance such as pitting or general corrosion.
—For Aluminum Association Class I and II architectural anodic coatings that are sealed in solutions containing less than 15 ppm silicates or 3 ppm phosphates, the acid pretreatment may be omitted.
1.4 In the case of coatings colored in deep shades, where estimation of the intensity of any residual dye stain is difficult, interpretation of the test is based on whether or not the original color has been affected by the action of the test.
1.5 This method is not applicable to:
1.5.1 Chromic acid type anodic coatings.
1.5.2 Anodic coatings on aluminum alloys containing more than 2 mass % Cu or 4.5 mass % Si.
1.5.3 Anodic coatings that have been sealed only in dichromate solutions.
1.5.4 Anodic coatings that have undergone a treatment to render them hydrophobic.
1.6 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of whoever uses this standard to consult and establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
ICS Number Code 25.220.20 (Surface treatment)
ASTM International is a member of CrossRef.
Citing ASTM Standards
[Back to Top]